2 Different types of carbon nanotubes, carbon nanofibers, vapor grown carbon fiber and other types of carbon nanostructure materials can be produced in various ways. In this section, different techniques for nanotube, nanofibers synthesis and their status are in brief described. The most common techniques used nowadays are: arc discharge, laser ablation, chemical vapour deposition. Economically feasible large-scale production and purification techniques still have to be developed.
3 In the arc discharge, a vapor is created by an arc discharge between two carbon electrodes with or without catalyst. In the laser ablation technology a high achievement laser beam, impose to a volume of the carbon, containing feedstock gas (methane or carbon monoxide). Now laser ablation produces a very small amount of pure nanotubes, while an arc-discharge method produces in general large amounts of the impure material. CVD seems to be the most promising method for possible industrial scale- up due to the relatively low growth temperature, high yields and high purities that can be achieved.
4 Arc dischargeThe carbon arc discharge method, initially used for producing C60 fullerenes, is the most common and perhaps easiest way to produce carbon nanotubes as it is rather simple to undertake. However, it is a technique that produces a mixture of components and requires separating nanotubes from the soot and the catalytic metals present in the crude product.
5 This method creates nanotubes through arc- vaporisation of two carbon rods placed end to end, separated by approximately 1mm, in an enclosure that is usually filled with inert gas (helium, argon) at low pressure (between 50 and 700 mbar). Recent investigations have shown that it is also possible to create nanotubes with the arc method in liquid nitrogen. A direct current of 50 to 100 A driven by approximately 20 V creates a high temperature discharge between the two electrodes °C. The discharge vaporises one of the carbon rods and forms a small rod shaped deposit on the other rod. Producing nanotubes in high yield depends on the uniformity of the plasma arc and the temperature of the deposit form on the carbon electrode
6 The Nanotubes created using this method are usually short tubes with diameters ranging from 0.6 to 1.4 nm for single walled and 10 nm diameter multi-walled nanotubes. These tubes can be single walled tubes or multiple walled nanotubes. This method is relatively easy to implement, and will produce yields of 30%. The nanotubes produced contain more impurities compared to other methods, and the consistency of the shape, wall, and lengths of the tubes are somewhat random [www.iljinnanotech.co.kr, and Journet and Bernier, 1998].
7 Figure 2.10 shows a schematic diagram of arc- discharge apparatus for the synthesis of carbon nanotubes. This apparatus must be connected both to a vacuum line with a diffusion pump, and to a helium supply. The electrodes are two graphite rods, usually of high purity. Typically, the anode is a long rod approximately 6 mm in diameter and the cathode a much shorter rod 9 mm in diameter. Efficient cooling of the cathode has been shown to be essential in producing good quality nanotubes [Iijima 1991; Ebbesen and Ajayan 1992; Ching-Hwa et al., 1995; Journet and Bernier, 1998; Jung et al., 2003].
9 Synthesis of SWNTIf SWNTs are preferable, the anode has to be doped with metal catalyst, such as Fe, Co, Ni, Y or Mo.A lot of elements and mixtures of elements have been tested by various authors16 and it is noted thatthe results vary a lot, even though they use the same elements. This is not surprising as experimental conditions differ.The quantity and quality of the nanotubes obtained depend on various parameters such as the metal concentration, inert gas pressure, kind of gas, the current and system geometry.Usually the diameter is in the range of 1.2 to 1.4 nm. A couple of ways to improve the process of arc discharge are stated below.
10 Inert gasThe most common problems with SWNT synthesis are that the product contains a lot of metal catalyst, SWNTs have defects and purification is hard to perform. On the other hand, an advantage is that the diameter can slightly be controlled by changing thermal transfer and diffusion, and hence condensation of atomic carbon and metals between the plasma and the vicinity of the cathode can control nanotube diameter in the arc process. This was shown in an experiment in which different mixtures of inert gases were used17. It appeared that argon, with a lower thermal conductivity and diffusion coefficient, gave SWNTs with a smaller diameter of approximately 1.2 nm. A linear fit of the average nanotube diameter showed a 0.2 nm diameter decrease per 10 % increase in argon helium ratio, when nickel/yttrium was used (C/Ni/Y was 94.8:4.2:1) as catalyst.
11 Optical plasma control A second way of control is plasma control by changing the anode to cathode distance (ACD). The ACD is adjusted in order to obtain strong visible vortices around the cathode. This enhances anode vaporisation, which improves nanotubes formation. Combined with controlling the argon-helium mixture, one can simultaneously control the acroscopic and microscopic parameters of the nanotubes formed18. With a nickel and yttrium catalyst (C/Ni/Y is 94.8:4.2:1) the optimum nanotube yield was found at a pressure of 660 mbar for pure helium and 100 mbar for pure argon. The nanotube diameter ranges from 1.27 to 1.37 nanometre.
12 CatalystKnowing that chemical vapour deposition (CVD) could give SWNTs with a diameter of 0.6–1.2 nm, researchers tried the same catalyst as used in CVD on arc discharge. Not all of the catalysts used appeared to result in nanotubes for both methods. But there seemed to be a correlation of diameter of SWNTs synthesised by CVD and arc discharge As a result, the diameter can be controllably lowered to a range of nm with arc-discharge. Using a mixture of Co and Mo in high concentrations as catalyst resulted in this result. These diameters are considerably smaller than nm16, which is the usual size gained from arcdischarge.
13 Improvement of oxidation resistance There is also progress in developing methods to improve the oxidation resistance of the SWNTs, which is a consequence of the defects present in nanotubes. A strong oxidation resistance is needed for the nanotubes if they have to be used for applications such as field emission displays. Recent research has indicated that a modified arc-discharge method using a bowl-like cathode (see Figure ), decreases the defects and gives cleaner nanotubes, and thus improves the oxidation resistance.
15 Open air synthesis with welding arc torch Only a couple of years ago, researchers discovered that it was possible to form MWNTs in open air 21. A welding arc torch was operated in open air and the process was shielded with an argon gas flow. The anode and cathode were made of graphite containing Ni and Y (Ni/Y is 4.2:1 at. %).This method was modified for preparing SWNTs22. A plate target made of graphite containing metal catalyst Ni and Y (Ni/Y is 3.6:0.8 at. per cent), was fixed at the sidewall of a water–cooled, steel based electrode.
16 The torch arc aimed at the edge of the target and the soot was deposited on the substrate behind the target (see Figure ). The arc was operated at a direct current of 100 A. and shielding argon gas flowed through the torch, enhancing the arc jet formation beyond the target.In the soot, carbon nanohorns (CNHs) and bundles of SWNT with an average diameter of 1.32 nm were found. However, the yield was much lower than for the conventional low- pressure arc discharge method. There are two reasons for this fact. At first, because of the open air, the lighter soot will escape into the atmosphere. Secondly, the carbon vapour might be oxidised and emitted as carbon dioxide gas. In order to improve the yield in this method, contrivances for collecting soot and development of an appropriate target are required.
18 Synthesis of MWNTIf both electrodes are graphite, the main product will be MWNTs. But next to MWNTs a lot of side products are formed such as fullerenes, amorphous carbon, and some graphite sheets. Purifying the MWNTs, means loss of structure and disorders the walls. However scientist are developing ways to gain pure MWNTs in a large- scale process without purification. Typical sizes for MWNTs are an inner diameter of 1-3 nm and an outer diameter of approximately 10nm. Because no catalyst is involved in this process, there is no need for a heavy acidic purification step. This means, the MWNT, can be synthesised with a low amount of defects.
19 Synthesis in liquid nitrogen A first, possibly economical route to highly crystalline MWNTs is the arc-discharge method in liquid nitrogen14, with this route mass production is also possible. For this option low pressures and expensive inert gasses are not needed.The content of the MWNTs can be as high as 70 % of the reaction product. Analysis with Augerspectroscopy revealed that no nitrogen was incorporated in the MWNTs. There is a strong possibility that SWNTs can be produced with the same apparatus under different conditions
21 Magnetic field synthesis Synthesis of MWNTs in a magnetic field gives defect-free and high purity MWNTs that can be applied as nanosized electric wires for device fabrication. In this case, the arc discharge synthesis was controlled by a magnetic field around the arc plasma.Extremely pure graphite rods (purity > %) were used as electrodes. Highly pure MWNTs (purity > 95 %) were obtained without further purification, which disorders walls of MWNTs
23 Figure 2-7: SEM images of MWNTs synthesised with (a) and without (b) the magnetic field.
24 Plasma rotating arc discharge A second possibly economical route to mass production of MWNTs is synthesis by plasma rotating arc discharge technique24. The centrifugal force caused by the rotation generates turbulence and accelerates the carbon vapour perpendicular to the anode. In addition, the rotation distributes the micro discharges uniformly and generates a stable plasma. Consequently, it increases the plasma volume and raises the plasma temperature.
25 At a rotation speed of 5000 rpm a yield of 60 % was found at a formation temperature of °C without the use of a catalyst. The yield increases up to 90% after purification if the rotation speed is increased and the temperature is enlarged to 1150 °C. The diameter size was not mentioned in this publication.